#------------------------------------------------------------------------------
#$Date: 2016-03-26 21:32:27 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180477 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/46/7214664.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7214664
loop_
_publ_author_name
'Wang, Xiuli'
'Xu, Chuang'
'Lin, Hongyan'
'Liu, Guocheng'
'Yang, Song'
'Gao, Qiang'
'Tian, Aixiang'
_publ_section_title
;
 Tuning the architectures of polyoxometalate-templated complexes by
 changing the spacer lengths of bis-pyridyl-bis-amide ligands (L): from 1D
 chains to 2D networks based on different (CuL)n loops
;
_journal_issue                   18
_journal_name_full               CrystEngComm
_journal_page_first              5836
_journal_paper_doi               10.1039/c2ce25371b
_journal_volume                  14
_journal_year                    2012
_chemical_formula_sum            'C42 H58 Cu2 Mo12 N12 O54 Si'
_chemical_formula_weight         2901.45
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                97.25(3)
_cell_angle_beta                 102.28(3)
_cell_angle_gamma                110.37(3)
_cell_formula_units_Z            1
_cell_length_a                   12.03(2)
_cell_length_b                   12.18(2)
_cell_length_c                   15.34(3)
_cell_measurement_temperature    293(2)
_cell_volume                     2009(6)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.983
_diffrn_measured_fraction_theta_max 0.983
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0332
_diffrn_reflns_av_sigmaI/netI    0.0737
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            9796
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.39
_exptl_absorpt_coefficient_mu    2.448
_exptl_absorpt_correction_T_max  0.6954
_exptl_absorpt_correction_T_min  0.6810
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.398
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1402
_exptl_crystal_size_max          0.17
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.16
_refine_diff_density_max         1.422
_refine_diff_density_min         -1.638
_refine_diff_density_rms         0.198
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     602
_refine_ls_number_reflns         6963
_refine_ls_number_restraints     14
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.0907
_refine_ls_R_factor_gt           0.0639
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0729P)²+17.1499P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1561
_refine_ls_wR_factor_ref         0.1745
_reflns_number_gt                5136
_reflns_number_total             6963
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2ce25371b.txt
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        2009(7)
_cod_database_code               7214664
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.22341(13) 0.47476(13) 1.30627(11) 0.0421(4) Uani 1 1 d . . .
Si1 Si 0.5000 1.0000 1.0000 0.0292(9) Uani 1 2 d S . .
Mo1 Mo 0.72877(9) 1.06360(9) 1.21081(7) 0.0348(3) Uani 1 1 d . . .
Mo2 Mo 0.40974(14) 0.89026(12) 1.18737(8) 0.0598(4) Uani 1 1 d U . .
Mo3 Mo 0.34788(14) 0.68360(9) 0.97757(7) 0.0557(4) Uani 1 1 d . . .
Mo4 Mo 0.68055(9) 0.82178(9) 1.02805(7) 0.0332(3) Uani 1 1 d . . .
Mo5 Mo 0.48862(11) 0.79463(9) 0.80652(7) 0.0455(3) Uani 1 1 d . . .
Mo6 Mo 0.82037(10) 1.12565(10) 1.01010(7) 0.0424(3) Uani 1 1 d . . .
O1 O 0.5368(11) 1.0351(12) 1.1133(8) 0.023(3) Uani 0.50 1 d P . .
O2 O 0.6243(12) 0.9948(12) 1.0453(9) 0.026(3) Uani 0.50 1 d P . .
O3 O 0.3785(12) 0.8906(11) 1.0276(8) 0.023(3) Uani 0.50 1 d P . .
O4 O 0.4859(12) 1.1268(11) 1.0333(8) 0.021(3) Uani 0.50 1 d P . .
O5 O 0.593(2) 0.9495(16) 1.2592(14) 0.050(3) Uani 0.509(17) 1 d PU A 1
O5' O 0.559(2) 0.9288(16) 1.2053(15) 0.050(3) Uani 0.491(17) 1 d PU A 2
O6 O 0.3432(14) 0.7181(13) 1.1165(9) 0.034(3) Uani 0.527(12) 1 d P A 1
O6' O 0.4203(16) 0.7803(15) 1.1109(11) 0.034(3) Uani 0.473(12) 1 d P A 2
O7 O 0.5431(16) 0.6901(14) 1.0227(11) 0.031(3) Uani 0.507(14) 1 d P A 1
O7' O 0.5163(17) 0.7352(15) 1.0294(12) 0.031(3) Uani 0.493(14) 1 d P A 2
O8 O 0.7268(8) 0.9053(8) 1.1476(6) 0.054(2) Uani 1 1 d . A .
O9 O 0.3877(16) 0.6604(13) 0.8587(10) 0.033(3) Uani 0.521(14) 1 d P A 1
O9' O 0.3629(17) 0.7116(14) 0.8720(11) 0.033(3) Uani 0.479(14) 1 d P A 2
O10 O 0.2521(14) 0.7512(13) 0.9547(10) 0.032(3) Uani 0.506(12) 1 d P . 1
O10' O 0.1775(15) 0.6962(14) 0.9634(10) 0.032(3) Uani 0.494(12) 1 d P . 2
O11 O 0.7988(9) 0.9704(7) 1.0025(6) 0.059(3) Uani 1 1 d . A .
O12 O 0.6363(15) 0.7679(15) 0.8855(10) 0.032(3) Uani 0.502(13) 1 d P A 1
O12' O 0.6035(15) 0.8139(15) 0.8958(10) 0.032(3) Uani 0.498(13) 1 d P A 2
O13 O 0.5724(11) 0.9374(10) 0.7798(11) 0.111(5) Uani 1 1 d . . .
O14 O 0.7185(13) 1.0889(12) 0.8966(9) 0.031(2) Uani 0.524(11) 1 d P . 1
O14' O 0.7916(15) 1.1467(14) 0.8849(10) 0.031(2) Uani 0.476(11) 1 d P . 2
O15 O 0.8263(9) 1.1377(7) 1.1441(6) 0.056(3) Uani 1 1 d . A .
O16 O 0.8311(12) 1.0843(8) 1.3106(6) 0.088(4) Uani 1 1 d . A .
O17 O 0.3531(8) 0.8438(8) 1.2751(5) 0.047(2) Uani 1 1 d . A .
O18 O 0.2823(7) 0.5360(7) 0.9740(6) 0.047(2) Uani 1 1 d . A .
O19 O 0.7677(12) 0.7389(10) 1.0349(7) 0.081(4) Uani 1 1 d . A .
O20 O 0.4652(9) 0.6888(9) 0.7147(6) 0.061(3) Uani 1 1 d . A .
O21 O 0.9716(9) 1.1967(9) 1.0225(7) 0.074(3) Uani 1 1 d . A .
O22 O -0.1915(8) 0.2396(9) 1.5271(7) 0.062(3) Uani 1 1 d . . .
O23 O 0.2491(9) 0.2906(10) 1.5645(6) 0.064(3) Uani 1 1 d . . .
O24 O 0.4756(8) 0.2367(8) 1.4779(6) 0.051(2) Uani 1 1 d . . .
O25 O 0.6683(10) 1.1768(10) 1.2379(10) 0.089(3) Uani 1 1 d U . .
N1 N 0.0609(9) 0.4333(9) 1.3426(7) 0.044(2) Uani 1 1 d . . .
N2 N 0.6222(9) 0.4787(9) 1.7369(7) 0.044(2) Uani 1 1 d . . .
N3 N -0.0069(9) 0.2258(10) 1.5396(7) 0.053(3) Uani 1 1 d . . .
H3B H 0.0598 0.2459 1.5227 0.063 Uiso 1 1 calc R . .
N4 N 0.2011(9) 0.1988(10) 1.6805(8) 0.054(3) Uani 1 1 d . . .
H4B H 0.2208 0.2035 1.7386 0.065 Uiso 1 1 calc R . .
N5 N 0.2114(9) 0.3050(9) 1.2952(7) 0.043(2) Uani 1 1 d . . .
N6 N 0.3659(9) 0.0366(9) 1.4424(7) 0.047(3) Uani 1 1 d . . .
H6A H 0.3013 -0.0219 1.4075 0.056 Uiso 1 1 calc R . .
C1 C 0.2980(9) 0.2788(11) 1.3565(8) 0.038(3) Uani 1 1 d . . .
H1A H 0.3610 0.3411 1.4010 0.045 Uiso 1 1 calc R . .
C2 C 0.1225(11) 0.2092(12) 1.2281(9) 0.050(3) Uani 1 1 d . . .
H2A H 0.0614 0.2234 1.1885 0.060 Uiso 1 1 calc R . .
C3 C 0.1199(11) 0.0946(12) 1.2169(9) 0.047(3) Uani 1 1 d . . .
H3A H 0.0634 0.0352 1.1672 0.056 Uiso 1 1 calc R . .
C4 C 0.2026(11) 0.0679(10) 1.2808(7) 0.038(3) Uani 1 1 d . . .
H4A H 0.1990 -0.0102 1.2766 0.046 Uiso 1 1 calc R . .
C5 C 0.2925(9) 0.1631(10) 1.3526(7) 0.029(2) Uani 1 1 d . . .
C6 C 0.3869(10) 0.1479(10) 1.4266(7) 0.034(3) Uani 1 1 d . . .
C7 C 0.4481(12) 0.0082(13) 1.5169(9) 0.053(3) Uani 1 1 d . . .
H7A H 0.4009 -0.0646 1.5335 0.064 Uiso 1 1 calc R . .
H7B H 0.4816 0.0732 1.5707 0.064 Uiso 1 1 calc R . .
C8 C 0.0415(10) 0.3690(11) 1.4069(8) 0.042(3) Uani 1 1 d . . .
H8A H 0.1016 0.3422 1.4332 0.050 Uiso 1 1 calc R . .
C9 C -0.0216(12) 0.4783(13) 1.3066(10) 0.056(4) Uani 1 1 d . . .
H9A H -0.0045 0.5281 1.2658 0.067 Uiso 1 1 calc R . .
C10 C -0.1364(12) 0.4499(13) 1.3308(12) 0.069(5) Uani 1 1 d . . .
H10A H -0.1961 0.4755 1.3020 0.083 Uiso 1 1 calc R . .
C11 C -0.1565(11) 0.3840(11) 1.3975(10) 0.051(3) Uani 1 1 d . . .
H11A H -0.2278 0.3688 1.4164 0.062 Uiso 1 1 calc R . .
C12 C -0.0677(10) 0.3405(10) 1.4360(8) 0.037(3) Uani 1 1 d . . .
C13 C -0.0909(10) 0.2659(11) 1.5053(8) 0.041(3) Uani 1 1 d . . .
C14 C -0.0219(14) 0.1486(16) 1.6054(11) 0.075(5) Uani 1 1 d . . .
H14A H -0.0998 0.0800 1.5814 0.090 Uiso 1 1 calc R . .
H14B H -0.0236 0.1928 1.6620 0.090 Uiso 1 1 calc R . .
C15 C 0.0837(14) 0.1048(14) 1.6246(12) 0.071(5) Uani 1 1 d . . .
H15A H 0.0615 0.0391 1.6557 0.086 Uiso 1 1 calc R . .
H15B H 0.0945 0.0740 1.5669 0.086 Uiso 1 1 calc R . .
C16 C 0.2821(13) 0.2804(12) 1.6450(9) 0.050(3) Uani 1 1 d . . .
C17 C 0.4020(11) 0.3650(11) 1.7128(8) 0.039(3) Uani 1 1 d . . .
C18 C 0.4123(12) 0.4148(12) 1.8034(8) 0.045(3) Uani 1 1 d . . .
H18A H 0.3429 0.3954 1.8252 0.054 Uiso 1 1 calc R . .
C19 C 0.5246(13) 0.4917(13) 1.8592(9) 0.054(3) Uani 1 1 d . . .
H19A H 0.5327 0.5217 1.9201 0.065 Uiso 1 1 calc R . .
C20 C 0.6306(12) 0.5266(12) 1.8241(9) 0.048(3) Uani 1 1 d . . .
H20A H 0.7058 0.5826 1.8616 0.058 Uiso 1 1 calc R . .
C21 C 0.5090(10) 0.4008(10) 1.6809(8) 0.034(3) Uani 1 1 d . . .
H21A H 0.5023 0.3706 1.6204 0.040 Uiso 1 1 calc R . .
O1W O 0.2483(9) 0.6480(8) 1.3378(6) 0.055(2) Uani 1 1 d . . .
O2W O 0.6528(8) 0.4758(8) 1.5133(6) 0.055(2) Uani 1 1 d . . .
O3W O 0.8997(12) 0.5378(12) 1.8527(8) 0.101(4) Uani 1 1 d . . .
O4W O 1.0073(19) 0.342(2) 1.8626(17) 0.230(13) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N5 Cu1 O1W 171.2(4) . .
N5 Cu1 N2 91.1(4) . 2_668
O1W Cu1 N2 90.0(4) . 2_668
N5 Cu1 N1 91.7(4) . .
O1W Cu1 N1 87.8(4) . .
N2 Cu1 N1 175.6(4) 2_668 .
O2 Si1 O2 179.997(7) 2_677 .
O2 Si1 O4 115.2(7) 2_677 2_677
O2 Si1 O4 64.8(7) . 2_677
O2 Si1 O4 64.8(7) 2_677 .
O2 Si1 O4 115.2(7) . .
O4 Si1 O4 179.998(8) 2_677 .
O2 Si1 O1 67.2(7) 2_677 2_677
O2 Si1 O1 112.8(7) . 2_677
O4 Si1 O1 70.6(6) 2_677 2_677
O4 Si1 O1 109.4(6) . 2_677
O2 Si1 O1 112.8(7) 2_677 .
O2 Si1 O1 67.2(7) . .
O4 Si1 O1 109.4(6) 2_677 .
O4 Si1 O1 70.6(6) . .
O1 Si1 O1 180.0(9) 2_677 .
O2 Si1 O3 69.7(7) 2_677 .
O2 Si1 O3 110.3(7) . .
O4 Si1 O3 75.9(6) 2_677 .
O4 Si1 O3 104.1(6) . .
O1 Si1 O3 104.0(6) 2_677 .
O1 Si1 O3 76.0(6) . .
O2 Si1 O3 110.3(7) 2_677 2_677
O2 Si1 O3 69.7(7) . 2_677
O4 Si1 O3 104.1(6) 2_677 2_677
O4 Si1 O3 75.9(6) . 2_677
O1 Si1 O3 76.0(6) 2_677 2_677
O1 Si1 O3 104.0(6) . 2_677
O3 Si1 O3 179.999(3) . 2_677
O16 Mo1 O15 102.2(6) . .
O16 Mo1 O25 101.3(6) . .
O15 Mo1 O25 98.8(5) . .
O16 Mo1 O8 98.5(4) . .
O15 Mo1 O8 88.2(4) . .
O25 Mo1 O8 157.1(5) . .
O16 Mo1 O5' 109.4(8) . .
O15 Mo1 O5' 145.0(7) . .
O25 Mo1 O5' 89.7(6) . .
O8 Mo1 O5' 72.8(6) . .
O16 Mo1 O5 88.5(8) . .
O15 Mo1 O5 166.7(7) . .
O25 Mo1 O5 86.6(6) . .
O8 Mo1 O5 82.4(6) . .
O5' Mo1 O5 22.1(6) . .
O16 Mo1 O1 156.4(6) . .
O15 Mo1 O1 98.6(5) . .
O25 Mo1 O1 64.2(6) . .
O8 Mo1 O1 93.2(4) . .
O5' Mo1 O1 54.9(7) . .
O5 Mo1 O1 72.7(7) . .
O16 Mo1 O2 158.8(5) . .
O15 Mo1 O2 68.3(4) . .
O25 Mo1 O2 99.0(5) . .
O8 Mo1 O2 63.3(4) . .
O5' Mo1 O2 76.8(7) . .
O5 Mo1 O2 98.9(7) . .
O1 Mo1 O2 43.0(4) . .
O5' Mo2 O17 115.1(8) . .
O5' Mo2 O6' 76.7(9) . .
O17 Mo2 O6' 115.4(6) . .
O5' Mo2 O14 136.5(8) . 2_677
O17 Mo2 O14 107.0(5) . 2_677
O6' Mo2 O14 95.0(7) . 2_677
O5' Mo2 O13 92.5(7) . 2_677
O17 Mo2 O13 97.1(5) . 2_677
O6' Mo2 O13 147.3(6) . 2_677
O14 Mo2 O13 71.6(6) 2_677 2_677
O5' Mo2 O6 101.8(8) . .
O17 Mo2 O6 90.6(5) . .
O6' Mo2 O6 29.6(6) . .
O14 Mo2 O6 87.5(6) 2_677 .
O13 Mo2 O6 159.1(6) 2_677 .
O5' Mo2 O5 21.5(6) . .
O17 Mo2 O5 95.5(6) . .
O6' Mo2 O5 92.8(8) . .
O14 Mo2 O5 150.1(6) 2_677 .
O13 Mo2 O5 86.5(6) 2_677 .
O6 Mo2 O5 112.2(6) . .
O5' Mo2 O14' 160.2(8) . 2_677
O17 Mo2 O14' 84.7(5) . 2_677
O6' Mo2 O14' 95.0(7) . 2_677
O14 Mo2 O14' 24.9(5) 2_677 2_677
O13 Mo2 O14' 84.9(5) 2_677 2_677
O6 Mo2 O14' 76.4(6) . 2_677
O5 Mo2 O14' 171.3(6) . 2_677
O5' Mo2 O3 92.7(8) . .
O17 Mo2 O3 149.9(4) . .
O6' Mo2 O3 57.8(6) . .
O14 Mo2 O3 49.8(5) 2_677 .
O13 Mo2 O3 92.7(5) 2_677 .
O6 Mo2 O3 71.6(5) . .
O5 Mo2 O3 113.6(6) . .
O14' Mo2 O3 67.8(5) 2_677 .
O5' Mo2 O1 56.1(7) . .
O17 Mo2 O1 155.4(4) . .
O6' Mo2 O1 86.2(6) . .
O14 Mo2 O1 81.0(5) 2_677 .
O13 Mo2 O1 62.7(4) 2_677 .
O6 Mo2 O1 113.2(5) . .
O5 Mo2 O1 70.7(6) . .
O14' Mo2 O1 105.9(5) 2_677 .
O3 Mo2 O1 51.4(5) . .
O10 Mo3 O18 115.6(6) . .
O10 Mo3 O9' 79.4(8) . .
O18 Mo3 O9' 112.1(6) . .
O10 Mo3 O7' 134.6(8) . .
O18 Mo3 O7' 108.5(6) . .
O9' Mo3 O7' 94.0(8) . .
O10 Mo3 O9 101.1(7) . .
O18 Mo3 O9 94.6(5) . .
O9' Mo3 O9 23.5(6) . .
O7' Mo3 O9 85.1(7) . .
O10 Mo3 O6' 92.1(7) . .
O18 Mo3 O6' 110.6(5) . .
O9' Mo3 O6' 135.8(7) . .
O7' Mo3 O6' 61.9(7) . .
O9 Mo3 O6' 143.0(7) . .
O10 Mo3 O10' 26.9(6) . .
O18 Mo3 O10' 89.9(5) . .
O9' Mo3 O10' 96.3(8) . .
O7' Mo3 O10' 153.6(7) . .
O9 Mo3 O10' 112.8(6) . .
O6' Mo3 O10' 94.4(6) . .
O10 Mo3 O6 87.3(6) . .
O18 Mo3 O6 88.5(5) . .
O9' Mo3 O6 158.8(7) . .
O7' Mo3 O6 83.6(7) . .
O9 Mo3 O6 168.7(6) . .
O6' Mo3 O6 27.5(5) . .
O10' Mo3 O6 78.1(6) . .
O10 Mo3 O7 150.6(7) . .
O18 Mo3 O7 93.6(5) . .
O9' Mo3 O7 92.7(8) . .
O7' Mo3 O7 16.9(5) . .
O9 Mo3 O7 78.0(7) . .
O6' Mo3 O7 73.9(6) . .
O10' Mo3 O7 168.3(6) . .
O6 Mo3 O7 90.9(6) . .
O10 Mo3 O3 50.2(6) . .
O18 Mo3 O3 153.0(4) . .
O9' Mo3 O3 89.2(6) . .
O7' Mo3 O3 85.2(6) . .
O9 Mo3 O3 110.0(5) . .
O6' Mo3 O3 54.7(5) . .
O10' Mo3 O3 70.8(5) . .
O6 Mo3 O3 69.6(5) . .
O7 Mo3 O3 102.0(5) . .
O19 Mo4 O7 91.0(7) . .
O19 Mo4 O8 101.6(5) . .
O7 Mo4 O8 103.1(6) . .
O19 Mo4 O7' 113.2(7) . .
O7 Mo4 O7' 22.6(5) . .
O8 Mo4 O7' 93.6(6) . .
O19 Mo4 O12' 110.0(6) . .
O7 Mo4 O12' 87.9(7) . .
O8 Mo4 O12' 146.4(6) . .
O7' Mo4 O12' 84.5(7) . .
O19 Mo4 O11 99.4(5) . .
O7 Mo4 O11 163.7(6) . .
O8 Mo4 O11 87.2(4) . .
O7' Mo4 O11 146.5(6) . .
O12' Mo4 O11 76.8(6) . .
O19 Mo4 O12 87.5(6) . .
O7 Mo4 O12 86.9(7) . .
O8 Mo4 O12 166.2(5) . .
O7' Mo4 O12 92.2(7) . .
O12' Mo4 O12 22.5(5) . .
O11 Mo4 O12 81.0(5) . .
O19 Mo4 O4 156.7(5) . 2_677
O7 Mo4 O4 75.5(6) . 2_677
O8 Mo4 O4 99.9(4) . 2_677
O7' Mo4 O4 56.4(6) . 2_677
O12' Mo4 O4 51.7(5) . 2_677
O11 Mo4 O4 90.4(5) . 2_677
O12 Mo4 O4 73.1(5) . 2_677
O19 Mo4 O2 160.2(6) . .
O7 Mo4 O2 106.7(6) . .
O8 Mo4 O2 66.4(4) . .
O7' Mo4 O2 84.2(6) . .
O12' Mo4 O2 80.0(6) . .
O11 Mo4 O2 65.5(4) . .
O12 Mo4 O2 101.9(5) . .
O4 Mo4 O2 41.8(4) 2_677 .
O12' Mo5 O20 115.9(7) . .
O12' Mo5 O13 92.6(8) . .
O20 Mo5 O13 105.1(6) . .
O12' Mo5 O25 145.5(7) . 2_677
O20 Mo5 O25 97.1(5) . 2_677
O13 Mo5 O25 87.7(5) . 2_677
O12' Mo5 O9 85.0(7) . .
O20 Mo5 O9 87.7(6) . .
O13 Mo5 O9 166.6(6) . .
O25 Mo5 O9 86.9(6) 2_677 .
O12' Mo5 O9' 90.9(8) . .
O20 Mo5 O9' 104.7(6) . .
O13 Mo5 O9' 144.8(6) . .
O25 Mo5 O9' 70.3(6) 2_677 .
O9 Mo5 O9' 22.7(5) . .
O12' Mo5 O12 21.4(6) . .
O20 Mo5 O12 94.5(6) . .
O13 Mo5 O12 99.4(6) . .
O25 Mo5 O12 164.3(6) 2_677 .
O9 Mo5 O12 83.1(7) . .
O9' Mo5 O12 96.6(7) . .
O12' Mo5 O1 88.5(7) . 2_677
O20 Mo5 O1 155.0(4) . 2_677
O13 Mo5 O1 66.0(5) . 2_677
O25 Mo5 O1 60.3(5) 2_677 2_677
O9 Mo5 O1 100.7(6) . 2_677
O9' Mo5 O1 79.0(6) . 2_677
O12 Mo5 O1 109.7(6) . 2_677
O12' Mo5 O4 52.0(6) . 2_677
O20 Mo5 O4 155.6(5) . 2_677
O13 Mo5 O4 97.0(6) . 2_677
O25 Mo5 O4 93.7(5) 2_677 2_677
O9 Mo5 O4 71.2(5) . 2_677
O9' Mo5 O4 58.9(6) . 2_677
O12 Mo5 O4 71.6(5) . 2_677
O1 Mo5 O4 46.2(4) 2_677 2_677
O21 Mo6 O11 104.2(5) . .
O21 Mo6 O14 117.0(6) . .
O11 Mo6 O14 90.5(5) . .
O21 Mo6 O14' 87.7(6) . .
O11 Mo6 O14' 105.6(5) . .
O14 Mo6 O14' 30.2(6) . .
O21 Mo6 O15 98.4(5) . .
O11 Mo6 O15 87.9(4) . .
O14 Mo6 O15 143.8(5) . .
O14' Mo6 O15 163.4(5) . .
O21 Mo6 O10 109.4(6) . 2_677
O11 Mo6 O10 143.0(5) . 2_677
O14 Mo6 O10 87.8(6) . 2_677
O14' Mo6 O10 90.9(6) . 2_677
O15 Mo6 O10 72.5(5) . 2_677
O21 Mo6 O10' 84.2(6) . 2_677
O11 Mo6 O10' 168.7(5) . 2_677
O14 Mo6 O10' 92.4(6) . 2_677
O14' Mo6 O10' 82.0(6) . 2_677
O15 Mo6 O10' 83.2(5) . 2_677
O10 Mo6 O10' 26.4(5) 2_677 2_677
O21 Mo6 O3 153.3(5) . 2_677
O11 Mo6 O3 100.8(4) . 2_677
O14 Mo6 O3 53.1(5) . 2_677
O14' Mo6 O3 76.5(6) . 2_677
O15 Mo6 O3 91.8(4) . 2_677
O10 Mo6 O3 50.6(5) 2_677 2_677
O10' Mo6 O3 72.5(5) 2_677 2_677
Si1 O1 O2 53.1(5) . .
Si1 O1 Mo1 124.7(6) . .
O2 O1 Mo1 72.0(6) . .
Si1 O1 Mo5 121.3(7) . 2_677
O2 O1 Mo5 143.1(8) . 2_677
Mo1 O1 Mo5 97.4(5) . 2_677
Si1 O1 Mo2 116.5(7) . .
O2 O1 Mo2 121.7(8) . .
Mo1 O1 Mo2 96.2(5) . .
Mo5 O1 Mo2 94.1(4) 2_677 .
Si1 O2 O4 60.6(6) . 2_677
Si1 O2 O1 59.7(6) . .
O4 O2 O1 101.6(9) 2_677 .
Si1 O2 Mo4 126.9(8) . .
O4 O2 Mo4 66.6(6) 2_677 .
O1 O2 Mo4 131.1(8) . .
Si1 O2 Mo1 124.3(7) . .
O4 O2 Mo1 141.5(8) 2_677 .
O1 O2 Mo1 65.0(6) . .
Mo4 O2 Mo1 94.3(4) . .
Si1 O3 Mo6 124.1(6) . 2_677
Si1 O3 Mo2 115.1(6) . .
Mo6 O3 Mo2 99.9(5) 2_677 .
Si1 O3 Mo3 116.6(6) . .
Mo6 O3 Mo3 99.9(5) 2_677 .
Mo2 O3 Mo3 96.4(4) . .
Si1 O4 O2 54.6(6) . 2_677
Si1 O4 Mo4 126.1(7) . 2_677
O2 O4 Mo4 71.6(6) 2_677 2_677
Si1 O4 Mo5 121.4(6) . 2_677
O2 O4 Mo5 132.6(8) 2_677 2_677
Mo4 O4 Mo5 97.0(4) 2_677 2_677
Mo2 O5 Mo1 120.0(10) . .
Mo2 O5' Mo1 146.7(11) . .
Mo2 O6 Mo3 119.1(7) . .
Mo2 O6' Mo3 142.8(9) . .
Mo4 O7 Mo3 123.2(8) . .
Mo3 O7' Mo4 150.2(10) . .
Mo4 O8 Mo1 135.4(5) . .
Mo3 O9 Mo5 125.0(7) . .
Mo3 O9' Mo5 142.8(10) . .
Mo3 O10 Mo6 152.3(9) . 2_677
Mo3 O10' Mo6 116.2(7) . 2_677
Mo6 O11 Mo4 137.9(5) . .
Mo5 O12 Mo4 118.2(7) . .
Mo5 O12' Mo4 154.8(10) . .
Mo5 O13 Mo2 137.1(6) . 2_677
Mo6 O14 Mo2 149.9(8) . 2_677
Mo6 O14' Mo2 114.8(7) . 2_677
Mo1 O15 Mo6 137.3(5) . .
Mo1 O25 Mo5 137.8(7) . 2_677
C8 N1 C9 120.1(11) . .
C8 N1 Cu1 120.0(7) . .
C9 N1 Cu1 119.7(9) . .
C20 N2 C21 118.8(11) . .
C20 N2 Cu1 118.8(9) . 2_668
C21 N2 Cu1 122.4(8) . 2_668
C13 N3 C14 122.8(11) . .
C16 N4 C15 123.6(12) . .
C2 N5 C1 116.5(10) . .
C2 N5 Cu1 123.9(8) . .
C1 N5 Cu1 119.6(8) . .
C6 N6 C7 124.4(11) . .
C5 C1 N5 121.8(11) . .
C3 C2 N5 123.6(11) . .
C2 C3 C4 119.5(12) . .
C3 C4 C5 118.4(11) . .
C1 C5 C4 119.9(10) . .
C1 C5 C6 115.7(10) . .
C4 C5 C6 124.4(10) . .
O24 C6 N6 120.5(10) . .
O24 C6 C5 120.9(10) . .
N6 C6 C5 118.2(10) . .
N6 C7 C7 109.0(14) . 2_658
N1 C8 C12 122.2(11) . .
N1 C9 C10 120.6(13) . .
C11 C10 C9 119.2(12) . .
C10 C11 C12 119.2(12) . .
C11 C12 C8 118.5(12) . .
C11 C12 C13 119.4(11) . .
C8 C12 C13 122.1(10) . .
O22 C13 N3 121.9(12) . .
O22 C13 C12 119.9(11) . .
N3 C13 C12 118.1(10) . .
N3 C14 C15 110.8(12) . .
N4 C15 C14 113.4(14) . .
O23 C16 N4 120.4(13) . .
O23 C16 C17 123.4(12) . .
N4 C16 C17 115.7(11) . .
C18 C17 C21 118.5(11) . .
C18 C17 C16 123.9(11) . .
C21 C17 C16 117.5(11) . .
C19 C18 C17 119.5(12) . .
C18 C19 C20 120.2(12) . .
N2 C20 C19 120.8(12) . .
N2 C21 C17 122.0(10) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 N5 2.004(11) .
Cu1 O1W 2.004(10) .
Cu1 N2 2.024(11) 2_668
Cu1 N1 2.058(11) .
Si1 O2 1.536(12) 2_677
Si1 O2 1.536(12) .
Si1 O4 1.641(13) 2_677
Si1 O4 1.641(13) .
Si1 O1 1.659(13) 2_677
Si1 O1 1.659(13) .
Si1 O3 1.773(13) .
Si1 O3 1.773(13) 2_677
Mo1 O16 1.675(9) .
Mo1 O15 1.802(9) .
Mo1 O25 1.812(10) .
Mo1 O8 2.035(9) .
Mo1 O5' 2.11(2) .
Mo1 O5 2.089(17) .
Mo1 O1 2.353(13) .
Mo1 O2 2.469(14) .
Mo2 O5' 1.64(2) .
Mo2 O17 1.706(8) .
Mo2 O6' 1.724(16) .
Mo2 O14 1.901(15) 2_677
Mo2 O13 2.018(11) 2_677
Mo2 O6 2.025(15) .
Mo2 O5 2.06(2) .
Mo2 O14' 2.296(17) 2_677
Mo2 O3 2.399(13) .
Mo2 O1 2.471(13) .
Mo3 O10 1.640(15) .
Mo3 O18 1.681(8) .
Mo3 O9' 1.730(17) .
Mo3 O7' 1.854(19) .
Mo3 O9 1.993(16) .
Mo3 O6' 2.060(17) .
Mo3 O10' 2.077(16) .
Mo3 O6 2.135(14) .
Mo3 O7 2.273(18) .
Mo3 O3 2.413(13) .
Mo4 O19 1.687(9) .
Mo4 O7 1.838(17) .
Mo4 O8 1.846(9) .
Mo4 O7' 1.895(19) .
Mo4 O12' 2.018(16) .
Mo4 O11 2.019(9) .
Mo4 O12 2.097(16) .
Mo4 O4 2.347(13) 2_677
Mo4 O2 2.428(14) .
Mo5 O12' 1.652(16) .
Mo5 O20 1.686(9) .
Mo5 O13 1.828(10) .
Mo5 O25 2.030(12) 2_677
Mo5 O9 2.037(15) .
Mo5 O9' 2.038(18) .
Mo5 O12 2.078(16) .
Mo5 O1 2.421(14) 2_677
Mo5 O4 2.435(13) 2_677
Mo6 O21 1.677(10) .
Mo6 O11 1.801(10) .
Mo6 O14 1.802(14) .
Mo6 O14' 1.944(15) .
Mo6 O15 2.026(10) .
Mo6 O10 2.051(15) 2_677
Mo6 O10' 2.146(16) 2_677
Mo6 O3 2.270(14) 2_677
O1 O2 1.770(18) .
O1 Mo5 2.421(14) 2_677
O2 O4 1.705(19) 2_677
O3 Mo6 2.270(14) 2_677
O4 O2 1.705(19) 2_677
O4 Mo4 2.347(13) 2_677
O4 Mo5 2.435(13) 2_677
O10 Mo6 2.051(15) 2_677
O10' Mo6 2.146(15) 2_677
O13 Mo2 2.018(11) 2_677
O14 Mo2 1.901(14) 2_677
O14' Mo2 2.296(17) 2_677
O22 C13 1.269(14) .
O23 C16 1.250(15) .
O24 C6 1.246(13) .
O25 Mo5 2.030(12) 2_677
N1 C8 1.345(15) .
N1 C9 1.347(15) .
N2 C20 1.358(15) .
N2 C21 1.374(15) .
N2 Cu1 2.024(11) 2_668
N3 C13 1.311(15) .
N3 C14 1.462(17) .
N4 C16 1.387(16) .
N4 C15 1.467(18) .
N5 C2 1.387(15) .
N5 C1 1.401(14) .
N6 C6 1.353(15) .
N6 C7 1.503(15) .
C1 C5 1.380(16) .
C2 C3 1.373(18) .
C3 C4 1.395(16) .
C4 C5 1.423(15) .
C5 C6 1.505(15) .
C7 C7 1.52(3) 2_658
C8 C12 1.421(16) .
C9 C10 1.44(2) .
C10 C11 1.39(2) .
C11 C12 1.405(17) .
C12 C13 1.492(17) .
C14 C15 1.53(2) .
C16 C17 1.510(18) .
C17 C18 1.406(17) .
C17 C21 1.420(15) .
C18 C19 1.364(18) .
C19 C20 1.438(18) .
